Enhanced Supercapacitor Performance Using Electropolymerization of Self-Doped Polyaniline on Carbon Film

In this work, we electrochemically deposited self-doped polyanilines (SPANI) on the surface of carbon-nanoparticle (CNP) film, enhancing the superficial faradic reactions in supercapacitors and thus improving their performance. SPANI was electrodeposited on the CNP-film employing electropolymerization of aniline (AN) and o-aminobenzene sulfonic acid (SAN) comonomers in solution. Here, SAN acts in dual roles of a self-doped monomer while it also provides an acidic environment which is suitable for electropolymerization. The performance of SPANI−CNP-based supercapacitors significantly depends upon the mole ratio of AN/SAN. Supercapacitor performance was investigated by using cyclic voltammetry (CV), galvanostatic charge and discharge (GCD), and electrochemical impedance spectroscopy (EIS). The optimal performance of SPANI−CNP-based supercapacitor exists at AN/SAN ratio of 1.0, having the specific capacitance of 273.3 Fg−1 at the charging current density of 0.5 Ag−1.


Introduction
Energy storage systems are important nowadays because of the growing requirement for high power in charging and discharging, and thus the development of supercapacitors has attracted extensive attention recently. Supercapacitors have been categorized into electrochemical double layer capacitors (EDLCs) and pseudocapacitors according to their mechanism of charge storage [1]. EDLCs store charge employing electrical double-layer electrostatic force in an electrochemical double layer (Helmholtz Layer) [2]. The main materials used in EDLC are carbon-based materials, such as graphene, carbon nanotubes, carbon black, etc. In pseudocapacitors, charge is stored via fast and reversible faradic reaction, which is based on electroactive materials with several oxidation and reduction states (e.g., metal oxides and conducting polymer). In general, the capacitance of pseudocapacitors are higher than EDLCs [3,4]. On the other hand, EDLCs use very stable carbons to increase voltage (V) [5,6].
Conducting polymers, such as polyaniline (PANI) which is a potential material for supercapacitors due to its excellent electrochemical activity, ease of synthesis, environmental stability, and high specific

Preparation of CNP Substrates
The carbon nanoparticle (CNP) electrodes were prepared by the following procedures. Graphite foil as the current collector was polished by sandpaper and washed by 0.05 M H 2 SO 4 , then dried in a vacuum oven at 120 • C for 2 h. Then, carbon nanoparticles and PVDF were mixed in a mass ratio of 9:1 by Agate mortar and dispersed in the NMP solvent, grinding until the paste was homogeneous. The paste was dropped onto a graphite foil (2 cm × 1 cm) and dried at 70 • C for 16 h in a vacuum oven. The loading mass of CNP was about 0.5 mg·cm −2 .

Preparation of SPANI−CNP Composite Electrodes
Monomers of AN and SAN was dissolved in 50 mL of distilled water with total concentration of 0.1 M at various mole ratio of AN/SAN from 0.5 to 4. SPANI was electrodeposited on CNP substrates forming SPANI−CNP composite electrodes using cyclic voltammetry in a three-electrode cell equipped with Pt counter electrode and reference electrode of Ag/AgCl. The potentials swept from −0.2 to Nanomaterials 2018, 8

Characterization Techniques
The surface morphology of the SPANI−CNP composites was identified by field-emission scanning electron microscopy (FE-SEM, JSM-6700F, JEOL Ltd., Tokyo, Japan). Infrared spectra were recorded on an FTIR spectrometer (Agilent Technologies, Cary 630, Santa Clara, CA, USA) to check the functional groups on polymer films. The structural and chemical composition were determined by X-ray photoelectron spectroscopy (XPS) using a Theta Probe AR-XPS (Theta 300 Version, Thermo Fisher Scientific, Paisley, UK) which scanned the surface of the sample with a monochromatic X-Ray beam source of 1486.6 eV (aluminum anode) and 15 kV.

Electrochemical Characterization
Electrochemical characterization of SPANI−CNP composite electrodes in the respective three-electrode cells and symmetric cells were analyzed using cyclic voltammetry (CV), galvanostatic charge and discharge (GCD), and electrochemical impedance spectroscopy (EIS) on an AUTOLAB PGSTAT302N electrochemical work station (Metrohm Autolab, Utrecht, Netherland). 1 N H 2 SO 4 was quoted as the electrolyte solution . Three-electrode cells were equipped with the SPANI−CNP working electrode, platinum plate counter electrode, and reference electrode of Ag/AgCl electrode, respectively. The cyclic voltammetry (CV) data were recorded with scan rates of 5 and 10 mV·s −1 over the potential window of −0.2-0.8 V in a three-electrode cell. In the symmetric cell, the CV data were obtained at various scan rates of 10, 25, 50, 75, 100, and 125 mV·s −1 over the potential window of 0-0.8 V. The galvanostatic charge-discharge (GCD) curves were obtained over the potential range of 0-0.6 V at various current densities of 0.5, 1, 1.5, 2, 2.5, 5, and 10 A·g −1 in symmetric devices. A current density of 1 and 5 A·g −1 was used in three-electrode experimental cells over the potential range of 0-0.8 V (vs. Ag/AgCl). The electrochemical impedance spectroscopy (EIS) measurements were carried out between the frequency range of 0.1 Hz to 100 kHz at an amplitude of 10 mV.

Cyclic Voltammograms of SPANI Electropolymerization on CNP Substrate
Electropolymerization of polyaniline needs attachment and chain extension between active intermediates of diradical dications [17] generated from the monomers and propagating oligomer chains. The diradical dication is an energetic electrophile, so polymerization is generally performed in the presence of a strong acid (e.g., 1 M HCl, pH = −0.15) to deposit polyaniline on the electrode. Because the SAN molecule has a sulfonic acid group (-SO 3 H) in the ortho-position on the benzene ring, SAN molecules can generate the diradical dications (the bipolaronic form of pernigraniline, presents peak at~800 mV in pH = −0.15) [18] through self-doping amino groups (-NH 2 on AN and SAN molecules). This species is an energetic electrophile, extracting an electron from AN and SAN and becoming a radical cation which bonds with another radical. The increase in the intensity of peak at 250 mV (in pH = −0.15) [18] indicates that these radical cations undergo bonding to form the polymer deposited on the substrate. Alternatively, we designed that the sulfonate-containing SAN mixed with AN as a comonomer to make a weakly acidic aqueous solution (pH = 5.0) without adding inorganic acid. Figure 1 shows the cyclic voltammogramms (CVs) of AN-SAN electropolymerization on a CNP substrate. In this weak acidic solution, the current still gradually increases with increasing the cycling number of electropolymerization, due to the increase in deposition of the conductive polymer. As above, when adding 1 M HCl to AN-SAN comonomers (pH= −0.15), the corresponding CVs of electropolymerization presented two distinct redox couples around at~250 mV and~800 mV [18]. But in this work (pH = 5.0), the above two peaks of diradical dications and radical cation are merged together to become indistinguishable in this weakly acidic environment.  Figure 2 shows the morphology of the CNP and SPANI−CNP composites. The CNP nanoparticles with the size of 20 nm can be seen in Figure 2a. The SPANI was assembled onto CNP film, thus enlarging the particle size to~50 nm as shown in Figure 2a,b. As compared the size of CNP nanoparticles, the increase of particle size of SPANI−CNP composites arises from assembling the SPANI deposition onto CNP particles having SPANI polymers acting as a wrapping layer.  benzenoid ring, respectively. The bands at 1204 cm −1 and 1304 cm −1 are assigned to C-H stretching vibration with aromatic conjugation [16]. benzenoid ring, respectively. The bands at 1204 cm −1 and 1304 cm −1 are assigned to C-H stretching vibration with aromatic conjugation [16]. In Figure 4, the atomic composition of the SPANI−CNP composites with different AN/SAN ratio is studied using X-ray photon spectroscopy (XPS), exhibiting the existence of C, N, O, and S elements. The N1s deconvolution of the SPANI−CNP composites with AN/SAN ratio of 1 and 4 are shown in Figure 5a,b. The binding energies of 399.2, 399.8, and 400.8 eV correspond to the imine (-N=), amine (-NH-), and polaron species (N + ), respectively [12]. The formation of polaron species is contributed by the nitrogen in the vicinity of H + cations when the polymers were self-doped with -SO3H groups on the polymer chains. The formation of imine sites is due to the strong hydrogen bonding of -NH to oxygen atoms. Table 1 lists the results of N1s deconvolution and doping degree ([N + ]/[N]), revealing the doping degree of SPANI−CNP composites with AN/SAN ratio of 1 higher than that with AN/SAN ratio of 4. This is because the former has a higher content of SAN compared to the latter. Based on previous report, the electrical conductivity of SPANI is proportional to the doping degree [16]. As a result, it is conceivable that the conductivity of SPANI−CNP composites with AN/SAN ratio of 1 is higher than that with AN/SAN ratio of 4.  In Figure 4, the atomic composition of the SPANI−CNP composites with different AN/SAN ratio is studied using X-ray photon spectroscopy (XPS), exhibiting the existence of C, N, O, and S elements. The N 1s deconvolution of the SPANI−CNP composites with AN/SAN ratio of 1 and 4 are shown in Figure 5a,b. The binding energies of 399.2, 399.8, and 400.8 eV correspond to the imine (-N=), amine (-NH-), and polaron species (N + ), respectively [12]. The formation of polaron species is contributed by the nitrogen in the vicinity of H + cations when the polymers were self-doped with -SO 3 H groups on the polymer chains. The formation of imine sites is due to the strong hydrogen bonding of -NH to oxygen atoms. Table 1 lists the results of N 1s deconvolution and doping degree ([N + ]/[N]), revealing the doping degree of SPANI−CNP composites with AN/SAN ratio of 1 higher than that with AN/SAN ratio of 4. This is because the former has a higher content of SAN compared to the latter. Based on previous report, the electrical conductivity of SPANI is proportional to the doping degree [16]. As a result, it is conceivable that the conductivity of SPANI−CNP composites with AN/SAN ratio of 1 is higher than that with AN/SAN ratio of 4. benzenoid ring, respectively. The bands at 1204 cm −1 and 1304 cm −1 are assigned to C-H stretching vibration with aromatic conjugation [16]. In Figure 4, the atomic composition of the SPANI−CNP composites with different AN/SAN ratio is studied using X-ray photon spectroscopy (XPS), exhibiting the existence of C, N, O, and S elements. The N1s deconvolution of the SPANI−CNP composites with AN/SAN ratio of 1 and 4 are shown in Figure 5a,b. The binding energies of 399.2, 399.8, and 400.8 eV correspond to the imine (-N=), amine (-NH-), and polaron species (N + ), respectively [12]. The formation of polaron species is contributed by the nitrogen in the vicinity of H + cations when the polymers were self-doped with -SO3H groups on the polymer chains. The formation of imine sites is due to the strong hydrogen bonding of -NH to oxygen atoms. Table 1 lists the results of N1s deconvolution and doping degree ([N + ]/[N]), revealing the doping degree of SPANI−CNP composites with AN/SAN ratio of 1 higher than that with AN/SAN ratio of 4. This is because the former has a higher content of SAN compared to the latter. Based on previous report, the electrical conductivity of SPANI is proportional to the doping degree [16]. As a result, it is conceivable that the conductivity of SPANI−CNP composites with AN/SAN ratio of 1 is higher than that with AN/SAN ratio of 4.

Electrochemical Studies
Electrochemical techniques of cyclic voltammetry (CV), electrochemical impedance spectroscopy (EIS), and galvanostatic charge-discharge were employed to study the performance of CNP and SPANI−CNP composite-based electrodes in a three-electrode cell and a symmetric cell, respectively. The specific capacitance value (C s ) of CNP-and SPANI−CNP composite-based electrodes can be calculated from the CV curves according to equation [8]: where m is the mass of the electroactive material (g), v is the sweep rate (V·s −1 ), ∆V is the potential range (V), and the integrated area under the CV curve I is the response current (A). According to Equation (1), the integrated area of CV curve is proportional to specific capacitance of electrodes, so the specific capacitance of the CNP electrode and SPANI−CNP composite electrodes with AN/SAN ratios of 0.5, 1.0, 2.3, and 4.0 were compared. Figure 6a,b shows the cyclic voltammograms (CVs) in a three-electrode cell at sweep rate of 5 and 10 mV·s −1 in 1 N H 2 SO 4 solution. In these CVs, the peaks of oxidation and reduction peaks were observed from the characteristics of SPANI. Figure 6a,b also indicate that the SPANI−CNP composite electrodes showed a higher specific capacitance and electrochemical performance as compared CNP electrode. Moreover, the SPANI−CNP composite electrode with AN/SAN ratio of 1.0 possessed the highest specific capacitance than other AN/SAN compositions. These could be attributed to higher electrical conductivity of SPANI and its Faradic contribution. Faradic contribution provided pseudocapacitance which was caused by reversible redox transition involving the exchange of protons (or cations) in the electrolyte (H 2 SO 4 ) explained as follows.
SPANI + H + + e − ↔ SPANI-H (2) where H + denotes the protons in the electrolyte (H2SO4). Protons come from the sulfonic acids of SAN units in polymer chains. This implies that the formation of more complete polaronic structure of SPANI chains at this case. The above equation suggests that both protons are involved in the redox process. Here, SPANI promotes faster charge-discharge rates through the Faradaic reaction arising from doping-dedoping of the self-doped groups of sulfonic acid in the SAN units. These results further indicate that charge stored at the surface of the SPANI from the pseudocapacitance storage mechanism is an important factor in achieving high gravimetric energy density values.   Figure 7c shows the CVs in a symmetric cell based on SPANI−CNP composite electrode supercapacitor with an AN/SAN ratio of 1.0 at scan rates of 10, 25, 50, 75, 100, and 125 mV•s −1 . These CVs have an almost rectangular shape from 10 mV•s −1 to 125 mV•s −1 , indicating fast transport of electrolyte ions and excellent capability. This represents that the charge transport on the surface of this electrode is highly efficient [9]. Figure 7d shows the CVs of the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 at various voltage windows, indicating that the shape of these CV curves remains almost identical in the potential range of 0.2 V to 1.0 V. This means that the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 has excellent capacitive characteristics and reversibility. The CVs exhibit a tail at the upper limit potential of 1.0 V, indicating the evolution of oxygen [9].
where H + denotes the protons in the electrolyte (H 2 SO 4 ). Protons come from the sulfonic acids of SAN units in polymer chains. This implies that the formation of more complete polaronic structure of SPANI chains at this case. The above equation suggests that both protons are involved in the redox process. Here, SPANI promotes faster charge-discharge rates through the Faradaic reaction arising from doping-dedoping of the self-doped groups of sulfonic acid in the SAN units. These results further indicate that charge stored at the surface of the SPANI from the pseudocapacitance storage mechanism is an important factor in achieving high gravimetric energy density values.    Figure 7c shows the CVs in a symmetric cell based on SPANI−CNP composite electrode supercapacitor with an AN/SAN ratio of 1.0 at scan rates of 10, 25, 50, 75, 100, and 125 mV•s −1 . These CVs have an almost rectangular shape from 10 mV•s −1 to 125 mV•s −1 , indicating fast transport of electrolyte ions and excellent capability. This represents that the charge transport on the surface of this electrode is highly efficient [9]. Figure 7d shows the CVs of the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 at various voltage windows, indicating that the shape of these CV curves remains almost identical in the potential range of 0.2 V to 1.0 V. This means that the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 has excellent capacitive characteristics and reversibility. The CVs exhibit a tail at the upper limit potential of 1.0 V, indicating the evolution of oxygen [9].   Figure 7c shows the CVs in a symmetric cell based on SPANI−CNP composite electrode supercapacitor with an AN/SAN ratio of 1.0 at scan rates of 10, 25, 50, 75, 100, and 125 mV·s −1 . These CVs have an almost rectangular shape from 10 mV·s −1 to 125 mV·s −1 , indicating fast transport of electrolyte ions and excellent capability. This represents that the charge transport on the surface of this electrode is highly efficient [9]. Figure 7d shows the CVs of the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 at various voltage windows, indicating that the shape of these CV curves remains almost identical in the potential range of 0.2 V to 1.0 V. This means that the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 has excellent capacitive characteristics and reversibility. The CVs exhibit a tail at the upper limit potential of 1.0 V, indicating the evolution of oxygen [9].

Electrochemical Impedance Spectroscopy
The interface behavior of the electrode materials in supercapacitors is usually studied using EIS analysis [15]. The EIS experiment was performed in the frequency range of 0.1 to 100 kHz at an amplitude of 10 mV. In Figure 8, the Nyquist plot of CNP and SPANI−CNP composite electrodes showed a semicircular arc in the high-frequency range and a straight line in the low-frequency range. The arc of the high-frequency range indicates the charge transfer limiting process arising from the double-layer capacitance coupled with the charge transfer resistance (Rct) at the contact interface between the electrode and electrolyte solution [10].  Table 2). The SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 exhibited the lowest Rct value among these SPANI−CNP composite electrodes, indicating that the SPANI composite with AN/SAN ratio of 1 has a relatively lower Rct and better capacitive behavior with small diffusion resistance [10]. On the other hand, the interception on the x-axis at the high-frequency region was used to estimate the equivalent series resistance (ESR). The ESR values can be obtained for the CNP and SPANI−CNP composite electrodes with AN/SAN ratios of 4.0, 2.3, 1.0, and 0.5 are 2.83, 2.9, 4.1, 2.39, and 3.23 Ω, respectively (refer to Table 2). The SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 exhibits the lowest ESR value. This situation could be attributed to the highest conductivity of SPANI with an AN/SAN ratio of 1.0 [16] and the incorporation of SPANI into the composite structure enhancing efficient transport of electrolyte ions to the surface of the composite electrodes. The SPANI polymer chains facilitate the attachment of H + ions for electrical neutrality. In the low-frequency region, the straight line corresponds to the Warburg resistance, which is caused by frequency dependence of ion diffusion and transport among the electrolyte to the electrode surfaces [10]. The almost vertical line of the SPANI−CNP composite electrode with an

Electrochemical Impedance Spectroscopy
The interface behavior of the electrode materials in supercapacitors is usually studied using EIS analysis [15]. The EIS experiment was performed in the frequency range of 0.1 to 100 kHz at an amplitude of 10 mV. In Figure 8, the Nyquist plot of CNP and SPANI−CNP composite electrodes showed a semicircular arc in the high-frequency range and a straight line in the low-frequency range. The arc of the high-frequency range indicates the charge transfer limiting process arising from the double-layer capacitance coupled with the charge transfer resistance (R ct ) at the contact interface between the electrode and electrolyte solution [10]. Figure 8 shows that the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 has the smallest diameter of the semicircular arc at the high-frequency region. The values of R ct for the CNP and SPANI−CNP composite electrodes with AN/SAN ratios of 0.5, 1.0, 2.3, and 4.0 are 1.0, 1.89, 1.63, 4.0, and 1.97, respectively (refer to Table 2). The SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 exhibited the lowest R ct value among these SPANI−CNP composite electrodes, indicating that the SPANI composite with AN/SAN ratio of 1 has a relatively lower R ct and better capacitive behavior with small diffusion resistance [10]. On the other hand, the interception on the x-axis at the high-frequency region was used to estimate the equivalent series resistance (ESR). The ESR values can be obtained for the CNP and SPANI−CNP composite electrodes with AN/SAN ratios of 4.0, 2.3, 1.0, and 0.5 are 2.83, 2.9, 4.1, 2.39, and 3.23 Ω, respectively (refer to Table 2). The SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 exhibits the lowest ESR value. This situation could be attributed to the highest conductivity of SPANI with an AN/SAN ratio of 1.0 [16] and the incorporation of SPANI into the composite structure enhancing efficient transport of electrolyte ions to the surface of the composite electrodes. The SPANI polymer chains facilitate the attachment of H + ions for electrical neutrality. In the low-frequency region, the straight line corresponds to the Warburg resistance, which is caused by frequency dependence of ion diffusion and transport among the electrolyte to the electrode surfaces [10]. The almost vertical line of the SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 in the low-frequency range indicates fast ion diffusion in the electrolyte and adsorption/desorption onto the electrode surface.

Galvanostatic Charge−Discharge
The specific capacitance of three-electrode and tow-electrode systems can be calculated from the galvanostatic charge-discharge curve at particular current densities by using Equations (3) and (4) [12], respectively: where I is the discharge current (mA), m is the mass of total electroactive material (g), ∆V is the potential range of charge and discharge, and ∆t is the discharge time (t). Figure 9 shows the galvanostatic charge and discharge curves of SPANI−CNP electrodes in a three-electrode system, where CNP and SPANI−CNP composites, platinum, and Ag/AgCl were used as the working electrode, the counter electrode, and the reference electrode, respectively, at a constant current density of 1 and 5 A·g −1 in 1 N H 2 SO 4 electrolyte solution within a potential window of 0-0.8 V. The charge and discharge curves on CNP electrodes have a symmetric triangular shape, indicating the behavior of an electrical double-layer capacitor (EDLC) [11]. But, a deviation from a straight line was shown in the galvanostatic charge-discharge curves of the SPANI−CNP composite electrodes, indicating pseudocapacitive behavior [14]. The SPANI−CNP composite electrode with an AN/SAN ratio of 1.0 exhibited the highest specific capacitance in these devices. Figure 10a shows the galvanostatic charge and discharge curves of SPANI−CNP electrodes in a symmetric cell at a constant current density of 1 A·g −1 in 1 N H 2 SO 4 electrolyte solution within a potential window of 0-0.6 V. The specific capacitances of the CNP and the SPANI−CNP-based supercapacitors in the symmetric cells with AN/SAN ratios of 0.5, 1.0, 2.3, and 4.0 are 68, 53.3, 213.3, 102.6 and 96.6 F·g −1 , respectively, at current density of 1 A·g −1 . The SPANI−CNP composite with an AN/SAN ratio of 1.0 had the highest specific capacitance among these symmetric cells. Figure 10b shows the discharging rate of SPANI−CNP composite with AN/SAN ratio of 1 at different current density, revealing that the discharging time increased with decreasing of the discharging current density. Figure 10c demonstrates the rate capability of CNP and SPANI−CNP-based capacitors, indicating that the specific capacitance decreases with increasing current density and the specific capacitance of the SPANI−CNP-based capacitor is higher than that of CNP-based capacitor.  Figure 10a shows the galvanostatic charge and discharge curves of SPANI−CNP electrodes in a symmetric cell at a constant current density of 1 A•g −1 in 1 N H2SO4 electrolyte solution within a potential window of 0-0.6 V. The specific capacitances of the CNP and the SPANI−CNP-based supercapacitors in the symmetric cells with AN/SAN ratios of 0.5, 1.0, 2.3, and 4.0 are 68, 53.3, 213.3, 102.6 and 96.6 F•g −1 , respectively, at current density of 1 A•g −1 . The SPANI−CNP composite with an AN/SAN ratio of 1.0 had the highest specific capacitance among these symmetric cells. Figure 10b shows the discharging rate of SPANI−CNP composite with AN/SAN ratio of 1 at different current density, revealing that the discharging time increased with decreasing of the discharging current density. Figure 10c demonstrates the rate capability of CNP and SPANI−CNP-based capacitors, indicating that the specific capacitance decreases with increasing current density and the specific capacitance of the SPANI−CNP-based capacitor is higher than that of CNP-based capacitor.   Specific energy density (E, Wh·kg −1 ) and specific power density (P, W·kg −1 ) can be calculated using the following equations [14]: where C s is the specific capacitance of the supercapacitors, V is the voltage range during the discharge process in galvanostatic charge and discharge curves, and t is the discharge time. Figure 10d shows the Ragone plot, indicating improvement in energy density (14.1 Wh/Kg) of SPANI−CNP-based capacitor with AN/SAN ratio of 1 as compared that (6.8 Wh/Kg) of CNP-based capacitor. This improvement in energy density can be attributed to the enhancement of effective cation diffusion in the SPANI−CNP composites. A SPANI−CNP-based supercapacitor with AN/SAN ratio of 1 was employed to test for the cycle stability though galvanostatic charge and discharge in current density of 2 A·g −1 for 5000 cycles. Figure 11 shows 96.1% retention in capacitance after 5000 cycles, indicating excellent cycle stability in this supercapacitor.

Conclusions
We electrodeposited self-doped polyaniline (SPANI) onto carbon nanoparticle (CNP) film to form a SPANI−CNP composite by electropolymerization and improved the capacitive performance of the CNP electrode through increasing its conductivity and psuedocapacitive characteristic. SPANI with AN/SAN ratio of 1 exhibited the best performance among these AN/SAN ratios. In galvanostatic charge and discharge, the SPANI−CNP composite with AN/SAN ratio of 1 exhibited maximum specific capacitance of 273.3 F·g −1 compared to 133.3 F·g −1 in the CNP electrode, the specific energy density and power density of SPANI−CNP composite with AN/SAN ratio of 1 were 7.3 Wh·Kg −1 and 5996.8 W·Kg −1 compared to 3.3 Wh·Kg −1 and 2997 W·Kg −1 for the CNP electrode. Moreover, the capacitance retention was 96.3% after 5000 cycles in galvanostatic charge and discharge. Our results have shown that the SAN can replace other external doping and have the same supercapacitive performance as polyaniline/carbon composites. The SPANI−CNP composite with AN/SAN ratio of 1 had a superior supercapacitive performance due to its Faradic contribution and its efficient charge-transfer and ion transport between electrolyte and electrode. These results demonstrated that the SPANI−CNP composites have practical potential for electrochemically stable supercapacitors.